|Year : 2019 | Volume
| Issue : 3 | Page : 118-121
Effect of chitosan on antibacterial activity of gypsum-based biomaterial compared to two dental liners
Hasan Subhi1, Ikhwan Hakimi2, Nicholas Thong Li Jie2, Fazal Reza3, Adam Husein3, Asma Abdullah Nurul4
1 Conservative Dentistry Unit, School of Dental Sciences, Universiti Sains Malaysia, Kelantan, Malaysia
2 School of Dental Sciences, Universiti Sains Malaysia, Kelantan, Malaysia
3 Biomaterials and Prosthodontics Unit, School of Dental Sciences, Universiti Sains Malaysia, Kelantan, Malaysia
4 School of Health Sciences, Universiti Sains Malaysia, Health Campus, 16150 Kubang Kerian, Kelantan, Malaysia
|Date of Web Publication||25-Jun-2019|
Dr. Asma Abdullah Nurul
School of Health Sciences, Universiti Sains Malaysia, Health Campus, 16150 Kubang Kerian, Kelantan
Dr. Hasan Subhi
Conservative Dentistry Unit, School of Dental Sciences, Universiti Sains Malaysia, Health campus, 16150 Kubang Kerian, Kelantan
Source of Support: None, Conflict of Interest: None
Aim: The aim of this in vitro study was to evaluate the antibacterial activity of gypsum-based biomaterial with different concentrations of chitosan (GP/CT) and to compare with the commercial dental materials, Dycal and glass ionomer cement (GIC) against the Streptococcus mutans. Materials and Methods: GP/CT was prepared with different concentrations of CT to GP of 0%, 10%, 20%, 40%, and 80% (w/w). The antibacterial study was carried out using agar diffusion method on Mueller-Hinton agar (MHA) against S. mutans. Uniform wells were prepared at equidistant points in the base layer of MHA. The wells were filled with the materials immediately after manipulation and preincubated for 2 h and then incubated. The means of inhibition zones were measured at 48 and 72 h. Results: The results revealed that higher means of inhibition zone were observed in a dose-dependent manner with higher concentrations of CT. GP/80%CT showed more effective antibacterial effect than GP/20%CT and GP/10%CT with significant degree and also with GP/40%CT with no significant result (P < 0.05), while GP/0%CT showed no inhibition of bacterial growth. GP/80%CT showed no statistically significant difference with GIC and Dycal on day 3. In addition, no significant bacterial growth inhibition was observed between GP/40%CT and GIC. Conclusion: Gypsum-based biomaterial has potent antibacterial activity against S. mutans when CT added. Higher antibacterial activity of GP/CT biomaterial was observed in a dose-dependent manner with higher concentrations of CT. GP/80%CT exhibits the antibacterial effect similar to that of Dycal and GIC.
Keywords: Antibacterial activity, Chitosan, Gypsum, Streptococcus mutans
|How to cite this article:|
Subhi H, Hakimi I, Jie NT, Reza F, Husein A, Nurul AA. Effect of chitosan on antibacterial activity of gypsum-based biomaterial compared to two dental liners. J Int Oral Health 2019;11:118-21
|How to cite this URL:|
Subhi H, Hakimi I, Jie NT, Reza F, Husein A, Nurul AA. Effect of chitosan on antibacterial activity of gypsum-based biomaterial compared to two dental liners. J Int Oral Health [serial online] 2019 [cited 2020 Jan 27];11:118-21. Available from: http://www.jioh.org/text.asp?2019/11/3/118/261261
| Introduction|| |
The main reason that contributes to the restoration failure in the dentistry is the existence of secondary caries., When fermentable carbohydrates are present, the plaque bacteria such as Streptococcus mutans invade and initiate a demineralization of tooth structure between the cavity wall and the restoration, leading to secondary caries formation. The antibacterial activity of the restorative materials inactivates the remaining bacteria and microleakage, preventing secondary caries formation, and provides a long-lasting restoration. Recently, the interests in enhancing the antibacterial properties of restorative materials are focused on incorporation of antibacterial agents in the composite.,,,
Chitosan (CT), a deacetylated derivative of chitin, is a naturally acquired polysaccharide obtained mainly from shrimp shells and crabs. CT is nontoxic, biocompatible, and has antibacterial activity., CT is highly desirable in the dental materials because of its antibacterial properties and biocompatibility. CT has been studied in many aspects of dentistry such as antibacterial agent in dental materials,, in dental tissue engineering,,, and as a component in toothpaste to reduce plaque formation and abrasion.,,
Gypsum “calcium sulfate” (GP) was used as a resorbable base material in this study. GP is safe, well tolerated, and has inherent osteoconductive properties. It can be employed to deliver pharmacologic agents, antibiotics, and growth factors., Thus, CT was incorporated into GP to synthesize a biocompatible antibacterial material for dental pulp lining.
The aim of the present study was to evaluate the effect of CT concentrations on the antibacterial activity of gypsum-based biomaterial against S. mutans by comparing with the commercial restorative materials, Dycal and GIC.
| Materials and Methods|| |
This experimental biological study was performed using agar diffusion method against the strain of S. mutans in three technical replicates and three independent biological experiments for each material group. All the culture procedures were conducted under sterile conditions.
The details of the materials used are listed in [Table 1]. Water-soluble CT chloride “referred to as CT in this study” was used. Calcium sulfate dihydrate was heated at 200°C for 5 h to convert it to hemihydrate form. GP/CT biomaterial was prepared with five different concentrations of CT to GP of 0%, 10%, 20%, 40%, and 80% (w/w). 250 mg of GP and CT powder was mixed with distilled water at a volume of 190, 200, 300, 400, and 600 μL, respectively, to obtain a moldable paste that sets in few minutes. Dycal and GIC were mixed according to the manufacturer's instructions.
Agar diffusion method
[Figure 1] shows the flowchart of the test procedures. The antibacterial activity of the test materials was evaluated using Mueller-Hinton agar (MHA). S. mutans (ATCC 35668) was cultured on blood agar at 37°C for 48 h in anaerobic environment; the bacteria were then harvested and suspended in Mueller-Hinton broth for overnight. The concentration was diluted to obtain a 0.5 McFarland turbidity standard (corresponding to 1.5 × 108 CFU/ml). Bacterial suspension was poured onto the MHA surface and the excess was extracted. Uniform wells (5 mm in diameter, 5 mm in height) were made at equidistant points in MHA with a sterile copper coil. The test materials were mixed on a sterile glass slab by a sterile spatula and placed immediately in the wells using a sterile amalgam carrier and condensed gently. Plates with and without inoculums incubated under the identical conditions and for the same period served as positive and negative controls.
The test materials were prediffused for 2 h at room temperature. Then, the plates were incubated in anaerobic condition at 37°C. The bacterial inhibition zones were evaluated after 48 and 72 h with a precision rule to the closest 0.5 mm. The results were represented as the mean and standard deviation.
Statistical analyses were performed using SPSS (Version 22.0; SPSS, Chicago, IL, USA). Statistical significance was evaluated by one-way analysis of variance followed by Dunnett's T3 post hoc test for multiple comparisons of each pair if there was a significant difference; P < 0.05 was considered statistically significant.
| Results|| |
The antibacterial activity of GP/CT, GIC, and Dycal against S. mutans is shown in [Figure 2] and [Figure 3]. Bacterial growth was observed in positive control, whereas no bacterial growth was observed in negative control. The test material showed antibacterial activity against S. mutans with different intensities when CT was added. Higher means of inhibition zones were observed in a dose-dependent manner with higher concentrations of CT.
|Figure 2: Antibacterial activity of GP/CT biomaterial, GIC, and Dycal. Values are expressed as mean ± standard deviation of diameter of inhibition zones in mm (n = 9). *P < 0.05 against GP/0%CT, #P < 0.05 against GP/10%CT, €P < 0.05 against GP/20%CT, ¥P < 0.05 against GP/40%CT, ₤P < 0.05 against GP/80%CT. GP/CT: Gypsum-based biomaterial; GIC: Glass ionomer cement|
Click here to view
|Figure 3: Inhibition zones promoted by GP/CT biomaterial, GIC, and Dycal against Streptococcus mutans. GP/CT: Gypsum-based biomaterial; GIC: Glass ionomer cement|
Click here to view
The results revealed that GP/80%CT biomaterial demonstrated no statistical significant with GIC and Dycal on day 3. However, no significant inhibition in the bacterial growth could be observed between GP/40%CT and GIC. In addition, GP/80%CT showed more effective antibacterial effect than GP/20%CT and GP/10%CT with significant inhibition (P < 0.05). However, no statistically significant was found between GP/40%CT and GP/20%CT, but GP/40%CT showed significant difference with GP/10%CT (P < 0.05). On the other hand, GP/0%CT showed no inhibition of bacterial growth.
| Discussion|| |
In the present study, we investigated the antibacterial activity of gypsum-based biomaterial with different concentrations of CT and compared that with Dycal and GIC. Although calcium sulfate has no antimicrobial activity, it is not a good material for the growth of some microbes, and it can be used as a scaffold to deliver therapeutic drugs and antibacterial agents; thus, it was applied as a resorbable scaffold to release the active antibacterial component of CT. S. mutans frequently implicated in dental caries and pulpal inflammation and has the main role in the initial lesion and pulpal pathology. The agar diffusion technique, a widely used method for the assessment of antimicrobial activity, was employed in this study. Many researchers have used this technique in antibacterial researches., However, some factors may interfere with the inhibition zone formation around the materials including strains of the bacteria, diffusion capacity of the antimicrobial agents, cellular density, agar medium, and anaerobic atmosphere.
The present study revealed that GP/CT biomaterial has potent antibacterial activity with a larger zone of bacterial growth inhibition in high concentration of CT, while pure gypsum was incapable to inhibit the growth of S. mutans.
The results showed that GP/80%CT had the highest inhibition zone among the experimental materials, but not to a significant degree with GP/40%CT. Both GP/80%CT and GP/40%CT showed antibacterial activity similar to that of GIC. However, Dycal showed higher antibacterial activity than GP/40%CT. The antibacterial efficacy of CT is related to the interaction between the amino groups of CT with a positive charge and the cell surfaces of the microbes with a negative charge. This interaction results in the leakage of proteinaceous and intracellular material due to the loss of the microbes' barrier function. The low CT concentration biomaterials (GP/10%CT and GP/20%CT) had the lowest antibacterial activity with significantly lower mean of inhibition zone than GP/80%CT. Fei Liu et al. stated that the antibacterial activity of CT in the medium increases when the CT concentration increases. As the bacterial inhibitory actions of CT depend on the amount of NH3+ and its strength is increased with higher NH3+ concentration, which is indicated by CT, the finding is comparable with the results obtained in our study. GP/0%CT did not show any activity against S. mutans, indicating that the antibacterial activity of the GP/CT biomaterial is related to the action of the CT.
Dental liners affect the bacterial growth by direct contact with the bacteria and diffusion into the dentinal tubules. In addition, the effect of dental liners on the bacterial growth originates from the antibacterial activity of the liner and/or the change of environmental conditions. Calcium hydroxide is an optimal medication for many clinical situations because of its antimicrobial action and stimulation of reparative dentin. It was shown in our results that Dycal had a strong antibacterial effect, confirming the results of others., This antibacterial effect may be related to the release of highly oxidant and free radicals hydroxyl ions, which shows extreme reactivity with several biomolecules. GIC is well known in its advantage to inhibit dental caries; the antibacterial activity of GIC is attributed to the low pH and fluoride release. The present study demonstrated that GP/CT biomaterial has potent antibacterial activity comparable with Dycal and GIC and the efficient of the bacterial inhibition varies significantly according to the concentration of CT.
The key strength of this study was the comparison of the synthesized materials with the commercial restorative materials – Dycal and GIC – which possess excellent antibacterial properties. However, this research was limited to one cariogenic bacterium and the evaluation of other cariogenic bacteria would be a fruitful area. This study is a brief attempt to evaluate the role of CT on gypsum-based biomaterial. Its effects against S. mutans are not a novelty, but the role of CT does provide a new treatment approach, which can be further researched.
| Conclusion|| |
Gypsum-based biomaterial has potent antibacterial activity against S. mutans, while pure GP did not show inhibition of bacterial growth. Higher antibacterial activity of GP/CT biomaterial was observed in a dose-dependent manner with higher concentrations of CT. Further experimental investigations are needed to access the antibacterial activity of GP/CT biomaterial against various bacteria involved in dental caries.
We would like to thank the staffs of Craniofacial Science Laboratory, School of Dental Sciences, Universiti Sains Malaysia, for their technical support.
Financial support and sponsorship
This study was supported by short-term grants, No. 304/PPSG/61313006 and No. 304/PPSG/61312099 of Universiti Sains Malaysia.
Conflicts of interest
There are no conflicts of interest.
| References|| |
Deligeorgi V, Mjör IA, Wilson NH. An overview of reasons for the placement and replacement of restorations. Prim Dent Care 2001;8:5-11.
Forss H, Widström E. Reasons for restorative therapy and the longevity of restorations in adults. Acta Odontol Scand 2004;62:82-6.
He J, Söderling E, Lassila LV, Vallittu PK. Incorporation of an antibacterial and radiopaque monomer in to dental resin system. Dent Mater 2012;28:e110-7.
Zhu W, Lao C, Luo S, Liu F, Huang Q, He J, et al.
Mechanical and antibacterial properties of benzothiazole-based dental resin materials. J Biomater Sci Polym Ed 2018;29:635-45.
Korkmaz FM, Tüzüner T, Baygin O, Buruk CK, Durkan R, Bagis B. Antibacterial activity, surface roughness, flexural strength, and solubility of conventional luting cements containing chlorhexidine diacetate/cetrimide mixtures. J Prosthet Dent 2013;110:107-15.
Chatzistavrou X, Fenno JC, Faulk D, Badylak S, Kasuga T, Boccaccini AR, et al.
Fabrication and characterization of bioactive and antibacterial composites for dental applications. Acta Biomater 2014;10:3723-32.
Uragami T, Yamamoto S, Miyata T. Dehydration from alcohols by polyion complex cross-linked chitosan composite membranes during evapomeation. Biomacromolecules 2003;4:137-44.
Ikinci G, Senel S, Akincibay H, Kaş S, Erciş S, Wilson CG, et al.
Effect of chitosan on a periodontal pathogen Porphyromonas gingivalis
. Int J Pharm 2002;235:121-7.
Chung YC, Wang HL, Chen YM, Li SL. Effect of abiotic factors on the antibacterial activity of chitosan against waterborne pathogens. Bioresour Technol 2003;88:179-84.
Travan A, Marsich E, Donati I, Benincasa M, Giazzon M, Felisari L, et al.
Silver-polysaccharide nanocomposite antimicrobial coatings for methacrylic thermosets. Acta Biomater 2011;7:337-46.
Elsaka SE. Antibacterial activity and adhesive properties of a chitosan-containing dental adhesive. Quintessence Int 2012;43:603-13.
Lee YM, Park YJ, Lee SJ, Ku Y, Han SB, Klokkevold PR, et al.
The bone regenerative effect of platelet-derived growth factor-BB delivered with a chitosan/tricalcium phosphate sponge carrier. J Periodontol 2000;71:418-24.
Akman AC, Tiǧli RS, Gümüşderelioǧlu M, Nohutcu RM. BFGF-loaded HA-chitosan: A promising scaffold for periodontal tissue engineering. J Biomed Mater Res A 2010;92:953-62.
Ge S, Zhao N, Wang L, Yu M, Liu H, Song A, et al.
Bone repair by periodontal ligament stem cellseeded nanohydroxyapatite-chitosan scaffold. Int J Nanomedicine 2012;7:5405-14.
Marsh PD. Dental plaque: Biological significance of a biofilm and community life-style. J Clin Periodontol 2005;32 Suppl 6:7-15.
Ganss C, von Hinckeldey J, Tolle A, Schulze K, Klimek J, Schlueter N. Efficacy of the stannous ion and a biopolymer in toothpastes on enamel erosion/abrasion. J Dent 2012;40:1036-43.
Schlueter N, Klimek J, Ganss C. Randomised in situ
study on the efficacy of a tin/chitosan toothpaste on erosive-abrasive enamel loss. Caries Res 2013;47:574-81.
Mamidwar S, Weiner M, Alexander H, Ricci J.In vivo
bone response to calcium sulfate/poly L-lactic acid composite. Implant Dent 2008;17:208-16.
Lazáry A, Balla B, Kósa JP, Bácsi K, Nagy Z, Takács I, et al.
Effect of gypsum on proliferation and differentiation of MC3T3-E1 mouse osteoblastic cells. Biomaterials 2007;28:393-9.
Thomas MV, Puleo DA. Calcium sulfate: Properties and clinical applications. J Biomed Mater Res B Appl Biomater 2009;88:597-610.
Rabea EI, Badawy ME, Stevens CV, Smagghe G, Steurbaut W. Chitosan as antimicrobial agent: Applications and mode of action. Biomacromolecules 2003;4:1457-65.
Hong SW, Baik JE, Kang SS, Yun CH, Seo DG, Han SH. Lipoteichoic acid of Streptococcus mutans
interacts with toll-like receptor 2 through the lipid moiety for induction of inflammatory mediators in murine macrophages. Mol Immunol 2014;57:284-91.
Hahn CL, Best AM, Tew JG. Cytokine induction by Streptococcus mutans
and pulpal pathogenesis. Infect Immun 2000;68:6785-9.
Torabinejad M, Hong CU, Pitt Ford TR, Kettering JD. Antibacterial effects of some root end filling materials. J Endod 1995;21:403-6.
Al-Hezaimi K, Al-Hamdan K, Naghshbandi J, Oglesby S, Simon JH, Rotstein I. Effect of white-colored mineral trioxide aggregate in different concentrations on Candida albicans in vitro
. J Endod 2005;31:684-6.
Bhavana V, Chaitanya KP, Gandi P, Patil J, Dola B, Reddy RB. Evaluation of antibacterial and antifungal activity of new calcium-based cement (Biodentine) compared to MTA and glass ionomer cement. J Conserv Dent 2015;18:44-6.
] [Full text]
Estrela C, Bammann LL, Estrela CR, Silva RS, Pécora JD. Antimicrobial and chemical study of MTA, Portland cement, calcium hydroxide paste, sealapex and dycal. Braz Dent J 2000;11:3-9.
Sabudin S, Derman M, Zainol I, Noorsal K.In vitro
cytotoxicity and cell seeding studies of a chitosan-silver composite for potential wound management applications. J Eng Sci 2012;8:29-37.
Fei Liu X, Lin Guan Y, Zhi Yang D, Li Z, De Yao K. Antibacterial action of chitosan and carboxymethylated chitosan. J Appl Polym Sci 2001;79:1324-35.
Lu Y, Liu T, Li H, Pi G. Histological evaluation of direct pulp capping with a self-etching adhesive and calcium hydroxide on human pulp tissue. Int Endod J 2008;41:643-50.
Poggio C, Arciola CR, Beltrami R, Monaco A, Dagna A, Lombardini M, et al.
Cytocompatibility and antibacterial properties of capping materials. ScientificWorldJournal 2014;2014:181945.
Poggio C, Beltrami R, Colombo M, Ceci M, Dagna A, Chiesa M.In vitro
antibacterial activity of different pulp capping materials. J Clin Exp Dent 2015;7:e584-8.
Freeman BA, Crapo JD. Biology of disease: Free radicals and tissue injury. Lab Invest 1982;47:412-26.
Vermeersch G, Leloup G, Delmée M, Vreven J. Antibacterial activity of glass-ionomer cements, compomers and resin composites: Relationship between acidity and material setting phase. J Oral Rehabil 2005;32:368-74.
[Figure 1], [Figure 2], [Figure 3]